Effect of Quaternary Ammonium Salt on Shear Bond Strength of
Orthodontic Brackets to Enamel
Hannaneh Ghadirian 1, Allahyar Geramy 2, Farhood Najafi 3, Soolmaz Heidari 4, Hamid Golshahi 5
1 Assistant Professor, Dental Research Center, Dentistry Research Institute, Tehran University of Medical Sciences, Tehran, Iran; Department of Orthodontics, School of Dentistry, Tehran University of Medical Sciences, Tehran, Iran
Professor, Dental Research Center, Dentistry Research Institute, Tehran University of Medical Sciences, Tehran, Iran; Department of Orthodontics,School of Dentistry, Tehran University of Medical Sciences, Tehran, Iran
3 Assistant Professor, Department of Resin and Additives, Institute for Color Science and Technology, Tehran, Iran 4
PhD Candidate, Department of Dental Biomaterials, School of Dentistry, Tehran University of Medical Sciences, Tehran, Iran 5
Postgraduate Student, Department of Orthodontics,School of Dentistry, Tehran University of Medical Sciences, Tehran, Iran
Objectives: This study sought to assess the effect of quaternary ammonium salt (QAS) on shear bond strength of orthodontic brackets to enamel.
Materials and Methods: In this in vitro experimental study, 0, 10, 20 and 30% concentrations of QAS were added to Transbond XT primer. Brackets were bonded to 60 premolar teeth using the afore-mentioned adhesive mixtures, and the shear bond strength of the four groups (n=15) was measured using a universal testing machine. After debonding, the adhesive remnant index (ARI) score was determined under a stereomicroscope. Data were analyzed using one-way ANOVA.
Results: The mean and standard deviation of shear bond strength of the control and 10%, 20% and 30% groups were 23.54±6.31, 21.81±2.82, 20.83±8.35 and 22.91±5.66 MPa, respectively. No significant difference was noted in shear bond strength of the groups (P=0.83). Study groups were not different in terms of ARI scores (P=0.80).
Conclusions: The results showed that addition of QAS to Transbond XT primer had no adverse effect on shear bond strength of orthodontic brackets.
Key words: Dental Enamel; Shear Strength; Transbond XT Light Cure Adhesive Primer
Journal of Dentistry, Tehran University of Medical Sciences, Tehran, Iran (2017; Vol. 14, No. 3)
H. Golshahi, Department of Orthodontics, Tehran University of Medical Sciences, Tehran, Iran
Received: 15 January 2017 Accepted: 25 April 2017
Prevention of enamel demineralization around orthodontic brackets is a challenge in orthodontic
treatment . Orthodontic brackets and
appliances complicate oral hygiene practice for patients and enhance the accumulation of dental plaque on tooth surfaces . Bracket bonding is routinely performed during fixed orthodontic treatment.
Despite numerous advantages, bracket bonding has a risk of debonding and plaque accumulation around brackets . Bracket debonding may occur during orthodontic treatment and increases the duration of treatment and cost and necessitates additional patient visits . Composite resins used for adhesive bracket bonding have a polymer matrix and
can provide a suitable environment for
proliferation of aerobic and anaerobic
Fig. 1: Teeth with acrylic blocks in molds
risk of occurrence of white spot lesions, this study aimed to assess the effect of QAS on shear bond strength of orthodontic brackets to enamel.
MATERIALS AND METHODS
In this in vitro, experimental study, sample size was calculated to be 12 in each of the four groups for assessment of shear bond strength according to a previous study by Li et al,  assuming alpha=0.05, beta=0.2, effect size of 0.57 and standard deviation of 2.5 using one-way ANOVA. The current investigation was approved by the ethics committee of Tehran University of Medical Sciences (IR.TUMS.REC 1395.2909). The QAS compound that was synthesized and used in this study was methacryloxyethyl cetyl dimethyl ammonium chloride, which was added to Transbond XT
light-cure adhesive primer (3M Unitek,
Monrovia, CA, USA) . Table 1 lists the constituents of primer and composite resin used in this study. A control group of pure primer was also considered.
The four study groups were as follows: 1. Control group containing pure primer
2. The 10% group, including 90wt% primer and 10wt% QAS
3. The 20% group, including 80wt% primer and 20wt% QAS
4. The 30% group, including 70wt% primer and 30wt% QAS
Different weight percentages were prepared using a digital scale (Santorius, Göttingen, Germany). For complete mixing, primer was incubated with QAS at 60°C for five minutes in an oven.
The containers were covered with foil to prevent light penetration. Next, the shear bond strength test was performed and the adhesive remnant index (ARI) score was determined.
Shear bond strength test:
Sixty sound first premolars extracted for orthodontic purposes with no caries, cracks or restorations were cleaned from soft tissue residues and immersed in 0.5% chloramine T solution at 4°C for seven days. The teeth were randomly divided into four groups of 15, rinsed and dried. Next, 32% phosphoric acid (Scotchbond Universal etchant; 3M ESPE, St. Paul, MN, USA) was used for etching of the enamel according to the manufacturer’s instructions. The teeth were etched for 15 seconds, rinsed and dried to obtain a chalky white appearance. The four types of primer were used for bracket bonding (control and 10%, 20% and 30% concentrations of QAS). Transbond XT composite (3M Unitek, Monrovia, CA, USA) was applied on standard stainless steel edgewise premolar bracket base (American Orthodontics, Sheboygan, USA) with 0.018-inch slot size according to the manufacturer’s instructions with
12.62 mm2 bracket base area. Brackets were then
bonded to the middle part of the buccal surface by applying equal force. After aligning the longitudinal axis of bracket parallel to the longitudinal axis of tooth, excess adhesive was removed by a scaler and light curing was performed using a light curing unit
with 1200 mW/cm2 intensity. Each tooth was cured
for 40 seconds from the mesial, distal, occlusal and gingival surfaces. All procedures were performed by the same operator. The samples were immersed in distilled water at 37°C for 24 hours.
Fig. 2: Universal testing machine
seconds and transfer time of 10 seconds . The teeth were then mounted in molds measuring 2.5x2.5 cm. The internal surface of the mold was coated with petroleum jelly and the teeth were fixed using 16x22 inch rectangular stainless steel ligature wire. Each tooth was positioned at the center of the mold and the rectangular wire was fixed to the mold using sticky wax so that the teeth remained fixed when applying acrylic resin. Auto-polymerizing acrylic resin was applied to the mold and the teeth were embedded in acrylic to the level
of their cementoenamel junction. After
polymerization of acrylic resin, the teeth in acrylic blocks were separated from the mold (Fig. 1). The shear bond strength test was performed in Tehran University Dental Research Center. Universal testing machine (Zwick Roell, Ulm, Germany) was used for shear bond strength testing. The teeth were placed in the machine such that the bracket base was parallel to the load application vector. Load was applied in occlusogingival direction at a crosshead speed of 0.5 mm/minute to the bracket-tooth interface (Fig. 2). Load at debonding was recorded in Newtons (N) and converted to Megapascals (MPa) by dividing the load in Newtons by the bracket base
surface area in square-millimeters (mm2).
Determination of ARI score:
After debonding, each tooth and debonded bracket were evaluated under a stereomicroscope (SMZ800, Nikon, Tokyo, Japan) at x10 magnification (Fig. 3). The ARI score was determined as follows:
Score 1. All adhesive remaining on the enamel surface Score 2. 90% of adhesive remaining on the enamel surface
Score 3. 10-90% of adhesive remaining on the enamel surface
Score 4. Less than 10% of adhesive remaining on the enamel surface
Score 5. No adhesive remaining on the enamel surface 
Results of shear bond strength:
The mean bond strength values of the four groups are presented in Table 2. As shown, the highest bond strength was noted in the control group and the lowest in 20% group. According to ANOVA, the difference in shear bond strength was not significant among the four groups (P=0.83). Results of ARI score:
Table 3 shows the results of ARI scores. The Kruskal Wallis test showed no significant difference among the groups in terms of ARI scores (P=0.80).
Table 1. Constituents of primer and composite resin used in this study
This study sought to assess the effect of addition of QAS to Transbond XT primer on shear bond strength of orthodontic brackets to the enamel. No significant difference was noted in shear bond strength of the groups. Study groups were not different in terms of ARI scores. Orthodontic brackets enhance plaque accumulation in the oral cavity  and white spot lesions develop in 50 to 75% of patients under fixed orthodontic treatment . Addition of antibacterial agents to composite resins and adhesives has been suggested as an effective approach for prevention of enamel demineralization during orthodontic treatment . QASs have been suggested for this purpose due to their confirmed antibacterial activity. However, the effect of addition of this compound on physical and mechanical properties of adhesives and composite resin should also be evaluated.
Table 2. Shear bond strength (MPa) of tested specimens in the four groups (n=15)
Group Minimum Maximum Mean Standard deviation
Control 11.89 37.63 23.54 6.31 10% 13.32 26.32 21.81 2.82 20% 4.87 35.96 20.83 8.35 30% 12.24 33.42 22.91 5.66
A previous study showed that addition of QAS to composite resin caused no change in shear bond strength of brackets after one month . This finding was in agreement with our results since we found no significant difference in shear bond strength of the groups containing QAS and the control group. No standard method exists for assessment of bracket bond strength to tooth structure because in the clinical setting, loads applied to brackets are complex and include a mixture of shear and tensile loads, which cannot be well simulated in vitro. However, shear bond strength test is often performed for this purpose  and was adopted in the current study as well. The results showed that by an increase in concentration of QAS, no significant reduction occurred in shear bond strength. Several factors affect the bracket bond strength to tooth structure including the type of adhesive, type of bracket, clinician’s expertise and patient’s cooperation .
Table 3. Adhesive remnant index (ARI) scores for the study groups
ARI score 1 2 3 4 5
Control 2 3 5 4 1
10% 3 3 3 4 2
20% 3 5 3 3 1
30% 2 3 4 4 2
Total 10 14 15 15 6
ARI: Adhesive remnant index
Product Constituents C.A.S No. By wt%
Primer (3M ESPE, St. Paul, MN, USA)
BisphonalA diglycidyl ether
dimethacrylate (Bis GMA) 1565-94-2 45-55 trade Secret Triethylene Glycol
Dimethacrylate 109-16-0 45-55 trade Secret Triphenylantimony 603-36-1 <1 trade Secret 4-
(Dimethylamino)-benzeneethanol 50438-75-0 <0.5 trade Secret Dl-camphorquinone 10373-78-1 <0.3 trade Secret Hydroquinone 123-31-9 <0.03 trade Secret
Composite (3M ESPE, Monrovia, CA, USA)
Silane Treated Quartz 100402-78-6 70-80 Bisphenol A Diglycidyl Ether
Dimethacrylate 1565-94-2 10-20
Bisphenol A Bis (2-Hydroxiethyl ether) Dimethacrylate
Extracted human premolars were used in this study, which are ideal for assessment of bond strength since they have smooth buccal and lingual surfaces. Our results showed that the shear bond strength in presence of all concentrations of QAS was higher than the acceptable threshold of 6-8 MPa . Thus, these concentrations may be used in the clinical setting with no adverse effect on bond strength, given that their other properties are also optimal for clinical use. This result was in agreement with that of Cheng et al.  who showed that addition of QAS to primer had no adverse effect on bond strength.
Zhang et al.  evaluated the effect of addition of silver nanoparticles and QAS to primer and adhesive and showed that addition of these compounds had no significant effect on bond strength and yielded a bond strength in the range of 30-35 MPa. However, Sodagar et al.  evaluated the addition of nano-chitosan particles to composite and showed that the composite containing 1% nano-chitosan had the highest and the composite containing 10% nano-chitosan had the lowest bond strength. They showed a reduction in bond strength by an increase in concentration of nano-chitosan particles. This result was in contrast to our findings, which may be due to the use of two different materials in the two studies. Poosti et al.  indicated that
addition of titanium oxide significantly
decreased the bond strength of composite to tooth structure. Their results were different from ours probably due to different materials used. Li et al.  evaluated the addition of QAS and silver
nanoparticles to orthodontic primer and
concluded that they had no adverse effect on bond strength. In this study, the effect of QAS on immediate bond strength was evaluated. Future studies are recommended to compare immediate and long-term bond strength after addition of QAS to orthodontic primer. Our study showed no significant difference in ARI scores of the four groups, which was in line with the results of a
previous study . However, our study had an in vitro design, and could not well simulate the clinical setting. In the oral environment, a combination of tensile, shear and torsional loads are applied and significant thermal changes, humidity, acidity and microbial plaque further complicate the situation, which cannot be ideally simulated in vitro. Thus, generalization of in vitro results to the clinical setting must be done with caution .
Within the limitations of this study, the results showed that QAS had no adverse effect on bond strength of orthodontic brackets to enamel.
1- Bishara SE, Ajlouni R, Soliman MM, Oonsombats C, Laffoon JF, Warren J. Evaluation of a new nano-filled restorative material for bonding orthodontic brackets. World J Orthod. 2007 Spring;8(1):8-12. 2- Van Waveren Hogervorst WL, Feilzer AJ, Prahl-Andersen B. The air-abrasion technique versus the
conventional acid-etching technique: A
quantification of surface enamel loss and a comparison of shear bond strength. Am J Orthod Dentofacial Orthop. 2000 Jan;117(1):20-6.
3- Powers JM, Kim HB, Turner DS, editors. Orthodontic adhesives and bond strength testing. Semin Orthod. Elsevier; 1997 Sep;3(3):147-56. 4- Brantley WA, Eliades T. Orthodontic materials: scientific and clinical aspects: J Orthod. 2002;29(1):75.
5- Kukleva MP, Shetkova DG, Beev VH. Comparative age study of the risk of demineralization during orthodontic treatment with brackets. Folia Med (Plovdiv). 2002;44(1-2):56-9.
6- Zhou H, Li F, Weir MD, Xu HH. Dental plaque microcosm response to bonding agents containing quaternary ammonium methacrylates with different chain lengths and charge densities. J Dent. 2013 Nov;41(11):1122-31.
ammonium and silver nanoparticles. J Dent Res. 2012 Jun;91(6):598-604.
8- Beyth N, Yudovin-Farber I, Bahir R, Domb AJ, Weiss EI. Antibacterial activity of dental composites containing quaternary ammonium polyethylenimine nanoparticles against Streptococcus mutans. Biomaterials. 2006 Jul;27(21):3995-4002.
9- Li F, Weir MD, Chen J, Xu HH. Comparison of quaternary ammonium-containing with nano-silver-containing adhesive in antibacterial properties and cytotoxicity. Dent Mater. 2013 Apr;29(4):450-61. 10- Ma S, Niu L, Li F, Fang M, Zhang L, Tay FR, et al. Adhesive materials with bioprotective/ biopromoting functions. Curr Oral Health Rep. 2014 Dec;1(4):213-21. 11- De Munck J, Van Landuyt K, Coutinho E, Poitevin A, Peumans M, Lambrechts P, et al. Micro-tensile bond strength of adhesives bonded to Class-I cavity-bottom dentin after thermo-cycling. Dent Mater. 2005 Nov;21(11):999-1007.
12- Oliver RG, Pal AD. Distortion of edgewise orthodontic brackets associated with methods of debonding. Am J Orthod Dentofacial Orthop. 1989 Jul;96(1):65-71.
13- Sudjalim TR, Woods MG, Manton DJ. Prevention of white spot lesions in orthodontic practice: a contemporary review. Aust Dent J. 2006 Dec;51(4):284-9.
14- Mota SM, Enoki C, Ito IY, Elias AM, Matsumoto MA. Streptococcus mutans counts in plaque adjacent to orthodontic brackets bonded with resin-modified glass ionomer cement or resin-based composite. Braz Oral Res. 2008 Jan-Mar;22(1):55-60.
15- Mirhashemi A, Bahador A, Kassaee M, Daryakenari G, Ahmad-Akhoundi M, Sodagar A. Antimicrobial effect of zinc oxide and nano-chitosan particles in dental composite used in orthodontics. J Med Bacteriol. 2015 Oct;2(3-4):1-0.
16- Hajrassie MK, Khier SE. In-vivo and in-vitro comparison of bond strengths of orthodontic brackets bonded to enamel and debonded at various times. Am J Orthod Dentofacial Orthop. 2007 Mar;131(3):384-90. 17- Cozza P, Martucci L, De Toffol L, Penco SI. Shear bond strength of metal brackets on enamel. Angle Orthod. 2006 Sep;76(5):851-6.
18- Cheng L, Weir MD, Zhang K, Arola DD, Zhou X, Xu HH. Dental primer and adhesive containing a new antibacterial quaternary ammonium monomer dimethylaminododecyl methacrylate. J Dent. 2013 Apr;41(4):345-55.
19- Zhang K, Melo MA, Cheng L, Weir MD, Bai Y, Xu HH. Effect of quaternary ammonium and silver nanoparticle-containing adhesives on dentin bond strength and dental plaque microcosm biofilms. Dent Mater. 2012 Aug;28(8):842-52.
20- Sodagar A, Bahador A, Pourhajibagher M, Ahmadi B, Baghaeian P. Effect of Addition of Curcumin Nanoparticles on Antimicrobial Property and Shear Bond Strength of Orthodontic Composite to Bovine Enamel. J Dent (Tehran). 2016 Sep;13(5):373-382.
21- Poosti M, Ramazanzadeh B, Zebarjad M, Javadzadeh P, Naderinasab M, Shakeri MT. Shear bond strength and antibacterial effects of orthodontic composite containing TiO2 nanoparticles. Eur J Orthod. 2013 Oct;35(5):676-9.
22- Akhavan A, Sodagar A, Mojtahedzadeh F, Sodagar K. Investigating the effect of incorporating nanosilver/nanohydroxyapatite particles on the shear bond strength of orthodontic adhesives. Acta Odontol Scand. 2013 Sep;71(5):1038-42.